Summary of the maximum dielectric constant and Curie temperature (TC) of PMN ceramics prepared from different methods, and piezoelectric properties of PMN-PT ceramics for different compositions (x) around the MPB.
Ferroelectric (1-x)[Pb(Mg1/3Nb2/3)O3]-xPbTiO3 (PMN-PT) solid solutions are known for their exceptional electromechanical properties, sometimes one order of magnitude larger than classical PbZr1-xTixO3 (PZT) ceramics. Prepared with a suitable x composition, PMN-PT is technologically important for fabricating some of the most important solid state devices such as a piezoelectric transducer, actuator, FERAM, etc. PMN-PT ceramics, thin films or single crystal forms can be prepared with high piezoelectric coefficients, a high dielectric constant and a low dielectric loss. Some compositions of PMN-PT single crystals exhibit a very high piezoelectric coefficient (d33) and electromechanical coupling coefficients (k33) (d33 ~ 1240 pC/N and k33 ~ 0.923), a high dielectric constant ( ~ 3100) with low dielectric loss (tan ~ 0.014) compared to those of polycrystalline ceramics (d33 ~ 690 pC/N and k33 ~ 0.73) (Park & Shrout, 1997; Viehland et al., 2001). Recently, researchers have also reported that PMN-PT single crystals have high remanent polarization (Pr ~ 35 C/cm2) at a low coercive field (Ec ~ 3.4 kV/cm), a high dielectric constant ( ~ 2500), low loss tangent (tan ~ 0.031), the highest piezoelectric coefficient (d33 ~ 1500 pC/N) and a high electrochemical coupling coefficient (k33 ~ 0.82) for <112> grain-oriented PMN–PT ceramics (Sun et al., 2004). The piezoelectric coefficient dij determines the stress levels induced by a given electric field and thus is the parameter most frequently used to describe the performance of an actuator.
PMN-PT solid solutions present a perovskite ABO3 structure, where the A site is occupied by the Pb2+ ion, while the B site is randomly occupied by Mg2+, Nb5+ and Ti4+ ions. Different compositions of the PMN-PT present distinct physical properties. The complex perovskite Pb(Mg1/3Nb2/3)O3 (x = 0) is a typical relaxor ferroelectric, characterized by a diffuse maximum of the dielectric constant associated with considerable frequency dispersion, that exhibits a non-polar paraelectric phase at high temperatures, similar in many aspects to normal ferroelectrics (Bokov & Ye, 2006). After cooling, a transformation occurs from the paraelectric phase to the ergodic relaxor state, characterized by the presence of polar nanoregions randomly distributed by the specimen, at the Burns temperature (
One of the most common problems related to PMN–PT emerges during synthesis. Indeed, obtaining high-density ceramics is very difficult without rigorous control of several steps in the processing, which makes using these materials for practical applications difficult. In the processing of PMN-PT solid solutions, the formation of an undesirable pyrochlore phase has long been recognized as a major problem for widespread use of these materials in the technology. In the last few years, several attempts, including modifications of the columbite method and other solid state reaction routes by using ultrafine powders, have been made to develop a processing technique in which formation of the pyrochlore phase is suppressed. Based on these processes, high-density ceramics could be obtained, and consequently, some properties could be improved. The purpose of this chapter is to provide an overview of the current understanding of some issues of the PMN-PT ferroelectric system at compositions around the MPB, including processing, structure and dielectric properties.
2. Processing and synthesis of PMN-PT
A major problem concerning the scientific studies and applications of PMN and PMN-PT electroceramics is the difficulty in producing a single-phase material with a perovskite structure. The main obstacle in PMN-PT synthesis is forming a lead niobate-based pyrochlore phase, frequently formed in the initial stage of the reactions processes for different methods. The presence of such a pyrochlore phase in the PMN-PT system is commonly believed to significantly degrade their dielectric properties, and therefore, the resulting material is inadequate for technological applications or a systematic scientific study (Mergen & Lee, 1997; Swartz & Shrout, 1982; Shrout & Swartz, 1983). Thus, choosing the synthesis method is fundamental to prepare pyrochlore-free PMN-PT of good quality. In general, several complex problems in materials science, such as the correct determination of the structure of the PZT solid solution in the MPB, remain unsolved in part due to the difficulty comparing results obtained from different samples. Some differences observed in peak widths of the neutron diffraction pattern suggest that the precise structural arrangements in these materials depend on the method of preparation (Yokota et al., 2009).
Compounds of the general formula A2B2O7 (A and B metals) represent a family of phases isostructural to the mineral pyrochlore (NaCa)(NbTa)O6F/(OH) (Subramanian, M.A. et al., 1983). Although A2B2O7 compounds exhibit a wide variety of interesting physical properties, in high-performance ferroelectrics such as PMN-PT these compounds should be avoided due to their paraelectric characteristic (Kamba et al., 2007). The compound Pb1.83Mg0.29Nb1.71O6.39 (PMN) exhibits a pyrochlore structure (space group Fd3m), frequently growing in the perovskite PMN ceramics, where the dielectric constant was found to increase as the temperature decreased, presenting an anomalous peak near 20 K, attributed to relaxation phenomena (Shrout & Swartz, 1983).
Chemical methods used to obtain complex precursor powders are normally less expensive and enable better stoichiometric control of complex oxides. Among several chemical methods, the approaches for obtaining mixed-cation oxide powders may be frequently grouped into two categories: the sol-gel process that uses alkoxide compounds as starting precursors (Johnson, 1985) and the polymeric precursor method that uses chelating agents such as citric acid (Lessing, 1989). In the sol-gel process, the high surface area of the dried gels results in high reactivity that in turn permits low temperature processing or even the formation of nonequilibrium phases. This process can be categorized in polymerized alkoxides and colloidal sols. The main advantages in using the polymerized alkoxides are low temperature, densification and ease doping compared to the disadvantage of slow drying. However,, colloidal sols present rapid drying and the low cost of the materials as advantages and doping difficulty as a disadvantage. In the popular polymeric precursor method, the synthesis of a cross-linked polymer resin provides some benefits such as homogeneous mixing of the cations and less tendency for segregation during calcinations. The main feature of the polymeric precursor method is that it allows a very homogeneous dispersion of the cations along the polymer. Thus, choosing a specific method to prepare mixed-cation oxide powders depends on several factors, including the kind of desired ceramic and the final objectives of each study.
Suppressing the pyrochlore phase is extremely difficult and depends on the synthesis method. To prepare pyrochlore-free PMN-PT ceramics or single crystals, several methods have been developed over the past three decades. The columbite process was known as a classical solid-state reaction method for synthesizing PMN (Swartz & Shrout, 1982). This method for solving the perovskite-pyrochlore reaction problem was proposed to bypass the formation of the intermediate pyrochlore phase reaction. By using the conventional mixed oxide technique and commercially starting materials, the following reaction sequences were proposed: MgO + Nb2O5 MgNb2O6 and MgNb2O6 + 3PbO 3(PMN). This procedure was adopted keeping in mind that the kinetics for liberating Nb2O5 from the MgNb2O6 columbite phase may be slow enough to prevent the pyrochlore phase from forming and that structure of the MgNb206 is a structure similar to the perovskite structure. At 900 °C, the reaction above is complete with small residuals of the pyrochlore phase. To remove this small amount of the pyrochlore phase, an MgO excess is introduced before the MgNb206 calcination step. Thus, powders with perovskite structure have been successfully synthesized with the two-step calcination technique described, where the columbite (MgNb2O6) phase is initially synthesized at 1000 °C and then reacts with PbO and TiO2 at 900 °C to form the pyrochlore-free PMN-PT phase. The effects of the MgO excess on the microstructure and dielectric properties of PMN and PMN-PT ceramics prepared by the columbite revealed that excess MgO completely inhibits formation of the pyrochlore phase and increases the grain size without substantially changing the density (Swartz et al., 1984). A significant increase in the dielectric constant values for PMN and PMN-PT, with x = 0.1, was observed with the addition of excess MgO and the increase in grain size and sintering temperature, reaching 18000 and 31000 for PMN and PMN-PT, respectively. Combining these factors to improve the dielectric constant in PMN-PT ceramics with the columbite method leads to a decrease at the Curie temperature (TC) as the grain size increases. These facts clearly indicate that the processing method plays an important role in the investigation of the phenomenology of ferroelectric ceramics based on the dielectric properties, since variations such as the TC shift are attributed to the clamping of domains walls or internal stresses generated at the grain boundaries (Randall et al., 1998). This method was also used to prepare PMN-PT ceramics compositions around the MPB, with a dense microstructure, grain size around 2-3 µm and excellent electromechanical properties (Kelly et al., 1997). In addition to the columbite method, routes such as coprecipitation (Sekar & Halliyal, 1998), sol-gel (Yoon et al., 1995), modified sol-gel (Babooram et al., 2004), combustion synthesis (Cruz et al., 2002), semi-wet chemical route (Panda & Sahoo, 2005) and others have been proposed to prepare pyrochlore-free PMN powders, which can be also extended to PMN-PT synthesis. Alternatively, methods that require only one calcination step to produce single-phase perovskite PMN–PT and PMN powders were also proposed (Gu et al., 2003). In this case, the Nb2O5 powder is coated with Mg(OH)2 in the first step, and in the second step, the Mg(OH)2-coated Nb2O5 powder is mixed with PbO for calcinations. The pyrochlore-free perovskite powders obtained could be sintered to almost full density at 1150 °C. The main advantage of this method over the columbite method is the single calcination step.
Variants of the columbite method were proposed to optimize their electrophysical properties or to be used as alternative routes to obtain fine powders. Often, oxide precursor powders with specific characteristics, with controlled particle size as an example, are not available commercially. An alternative for each research laboratory is producing its own power with the desired characteristic. Thus, variants of the processes already established have arisen. A variant is the polymerized complex method based on the Pechini-type reaction route (Pechini, 1967). The general idea of this approach is to distribute the metallic ions homogeneously throughout the polymeric resin, in which chelate is formed between dissolved ions and a hydroxycarboxylic acid (citric acid is the usual). Heating the resin in air causes a breakdown of the polymer, and subsequent calcinations at 500 to 900 °C are necessary to form the desired mixed oxides (Lessing, 1989). This alternative was also applied to produce MgNb2O6 powders, which were used as precursors to produce the PMN phase, obtained by the solid-state reaction between MgNb2O6 and PbO (Guarany, 2006; Guerra et al., 2009).
The polymerized based on the Pechini method combined with the columbite method was also applied to obtain good-quality PMN-PT ceramics at compositions around the MPB with a tendency to <111>-orientation (Araújo et al., 2007). The texture tendency observed in these ceramics was attributed to shear rates introduced during the ceramic pressing when a fine powder was used. Similar <112> and <001> grain-oriented PMN-PT ceramics, at x = 0.30 and 0.32, respectively. The first one was prepared with a directional solidification method of the compressed powders prepared by the columbite method (Sun et al., 2004), and the second ceramic was produced with the templated grain growth method (Sabolsky et al., 2001). The latter method, responsible for synthesizing PMN-PT ceramics with good-quality texture, is a processing routine that uses a tabular (001)-oriented SrTiO3 as a template (Kwon et al., 2005), at which the volume fraction of the oriented material increases as the thermal treatment continues at the expense of the finer grain matrix (Kwon et al., 2005). Despite the different methods proposed in the literature, studies of the phenomenology behind the MPB often have used ceramics prepared with the columbite classic method or some variation thereof. Table 1 summarizes the physical, dielectric and piezoelectric properties of PMN and PMN-PT ceramics for different compositions (x) around the MPB.
|References||Kmax (at 1 kHz)||TC (°C)||Comments|
|Swartz et al. (1984)||16200||-10||Columbite method|
|Wang & Schulze (1990)||13700||-10||Modified columbite method|
|Kong et al. (2001)||13979||-||High-energy ball milling|
|Panda & Sahoo (2005)||10335||-||Semi-wet chemical route|
|Paula et al. (2008)||19000||-6||Modified columbite method|
|Sun et al. (2004)||0.30||~1500||0.82||0.51||<112"/> Grain-oriented ceramics|
|Sabolsky et al. (2001)||0.32||~1200||0.755||-||<001"/> Textured ceramics|
|Kelly et al. (1997)||0.30|
|Park et al. (1997)||0.30|
|Poled and unpoled ceramics|
The preparation method also has a strong influence on the microstructure and dielectric properties of ferroelectric ceramics. In general, chemical methods that produce fine powders are more favorable for producing PMN-PT ceramics with a dense microstructure and larger grain size, but the density and grain size both depend on the sintering temperature. For ceramics prepared with the columbite method, the density decreases as the sintering temperature increases while the grain size increases (Swartz et al., 1984; Kong et al., 2001). An increase in the dielectric constant as the sintering temperature increases has also been observed for different compositions of PMN-PT (Baek et al., 1997). Grain-size dependence of the dielectric constant of PMN-PT ceramics was observed in the ferroelectric and paraelectric region, and this observation indicates that it is not a domain or stress effect (Swartz et al., 1984).
3. Structure of PMN-PT compositions at the MPB
The highest piezoelectric and electromechanical coupling coefficients of the PMN-PT (Park & Shrout, 1997) are found for compositions in the MPB at 0.27 < x < 0.37, between the tetragonal and rhombohedral regions of the x-T phase diagram (Noblanc et al., 1996). A typical example of the MPB between the tetragonal and rhombohedral perovskite phases can be found in the x-T phase diagram of the PZT system at around x ≈ 0.52 (Jaffe et al., 1971), where the highest piezoelectric coefficients are also observed. Since the 1970s, the MPB has been interpreted in terms of different models that attempt to explain the high piezoelectric response in the PZT system. The assumption that the morphotropic phase change is a first-order transition that defines a finite region where both tetragonal and rhombohedral phases coexists was one of the most discussed models (Arigur & Benguigui, 1975) until the mid-1990s (Mishra et al., 1996). The assumption of a metastable character for one of the two phases within the finite coexistence region (Isupov, 1975) and the propose of a true boundary explained with compositional fluctuations (Kakegawa & Mohri, 1977) were other models considered to understand the nature of the MPB in the PZT system. As often happens in science, complicated models reflect the degree of difficulty in understanding a problem, and new paradigms must be considered. These models began to decline when a study published in 1998 (Du et al., 1998), based on the phenomenological approach, revealed a great enhancement of piezoelectric coefficient
The discovery of a stable monoclinic phase in the PZT system in 1999, at compositions in the MPB (Noheda et al., 1999, 2000, 2001), provides a new perspective for explaining the high piezoelectric response of PZT ceramics (Guo et al. 2000, Singh et al. 2008, Bellaiche et al. 2000), attributed before to the coexistence of tetragonal and rhombohedral phases. After the initial discovery of a monoclinic phase with space group
Ferroelectric solid solutions exhibit high piezoelectric and electromechanical coupling coefficients and high dielectric permittivity at compositions in the MPB. But, what is the real importance of the monoclinic phases on the physical properties of these systems? Since the discovery of a monoclinic phase in PZT and PMN-PT solid solutions, several works have been published to understand the mechanisms responsible for the high piezoelectric response of these materials. The discovery of the monoclinic phases in these systems has catalyzed several exciting experimental (Guo et al., 2000; Bokov & Ye, 2004; Viehland et al., 2004) and theoretical developments (Fu & Cohen, 2000; Vanderbilt & Cohen, 2001). Interesting field-induced phase transitions were discovered in PMN-PT (Chen et al., 2002; Zhao et al., 2003), highlighting the important role of the intermediate monoclinic phase for the large electromechanical response of this material. Theoretical first principles calculations and phenomenological theory considerations have not only confirmed the existence of monoclinic phases in the MPB region but also revealed the dominant role of the rotational instabilities of the polarization vector across the MPB compositions (Fu & Cohen, 2000; Vanderbilt & Cohen, 2001). Further, phenomenological theory considerations have shown that the Devonshire free energy expansion up to the eighth-order term is needed to stabilize the monoclinic phases, indicating the highly anharmonic nature of these materials (Vanderbilt & Cohen, 2001). All these studies have also led to significant modifications of the x-T phase diagrams of these solid solutions (Noheda et al., 2002), including the phase diagram of the PMN-PT system, previously established by Noblanc et al. (Noblanc et al., 1996) and Choi et al. (Choi et al., 1989). Thus, based on these results, a new x-T phase diagram for PMN-PT near the MPB could be constructed, as shown in Fig. 1-(A) with the shaded area.
The monoclinic phase with the
In the above paragraphs, the monoclinic phases
The observed phases and phase transition in barium titanate, BaTiO3 and ferroelectrics in general were explained by Devonshire (Devonshire, Phil Mag 40, 1040 1949) in terms of the phenomenological Landau theory, based on a sixth-order expansion of the free energy in terms of order parameter P. However, the sixth-order Devonshire expansion fails to describe the existence of the monoclinic phase MA observed initially in the PZT system. A work published in 2000 (Souza et al., 2000) confirms that the Devonshire phenomenological theory is not adequate for predicting the observed monoclinic phase. Then, Vanderbilt and Cohen (Vanderbilt & Cohen, 2001) showed that the simplest extension of the Devonshire theory, including an eighth-order term in the ferroelectric order parameter, admits the monoclinic phases MA, MB and MC. An extension of the model to a twelfth-order term also predicts a triclinic ferroelectric phase.
3.1. Structural phase transition near the MPB: temperature-dependence
In addition to the complexity interpretation of the PMN-PT transformations for different compositions, the temperature dependence of the structural phase transitions in the MPB is another challenge. Several efforts have been made in the past few years to solve the phase transition problem for the PMN-PT system near the MPB, including structural studies conducted with high-resolution X-ray diffraction, spectroscopic studies (Araújo et al., 2008; Hlinka et al., 2006a) and dielectric analysis (Li et al., 2006; Hlinka et al., 2006b).
Spectroscopic techniques, such as Raman and infrared spectroscopy (IR), are useful tools for investigating phase transitions in polycrystalline materials and single crystals. Infrared spectroscopy can be used to study ferroelectric phase transitions since infrared vibrational frequencies, and consequently the interatomic forces, are affected by the onset of the ferroelectric state due to the temperature phase transitions. In the infrared spectra of the PMN-PT at composition x = 0.35, a broad band is observed from 472 cm-1 to 870 cm-1 (Araújo et al., 2008). This band is associated with 1-(Nb-O), 1-(Ti-O) and 1-(Mg-O) stretching modes in the PMN-PT structure. The IR curve shape changes slightly when the temperature increases, and these discrete changes as a function of the temperature may be attributed to the phase transitions involved in this system, introduced by distortions in BO6 octahedra. Considering that an observed infrared spectrum for PMN-PT is a composition of the stretching modes in the BO6 octahedron, each IR spectrum, recorded for different temperatures, can be fitted by considering three lorentzian functions:
The shift for lower frequencies of 1-stretching modes, as a function of increasing temperature (nonlinear behavior), can be explained by the inverse relationship between atomic separation and vibrational frequency if there is no structural phase transition in the observed temperature range. If we consider that the vibrational amplitude is proportional to the increasing temperature (), then the nonlinear case described by the restoring force can be written as follows:
where k is the corresponding force constant and represents the departure from linearity. Expanding as a power series in equation (2) and solving the differential equation with the successive approximations method, the wavenumber can be expressed as:
in which C
The phase transitions for the PMN-PT system by using IR spectroscopy can be understood from the point of view of the group representation, considering the possible symmetries involving the BO6 octahedron. The cubic symmetry, point group O
Under the above considerations, the monoclinic and tetragonal phase coexistence in PMN-PT must be interpreted as a superposing of two double partially degenerate band structures. Considering that these bands occur at very close frequencies, using three lorentzian functions is sufficient to fit each IR spectrum by using Equation (1). To illustrate this discussion, Fig. 2 shows the behavior of the 1-(Ti-O) mode as a function of temperature, obtained from the PMN-PT single crystal for composition x = 0.35 (Araújo et al., 2008). The singularities observed at around 230 K, 300 K and 422 K were interpreted as the result of structural phase transitions induced by the temperature increase while the curves in this figure represent the theoretical fitting of the experimental data by using Equation (3). The anomalous behavior observed for the 1-(Ti-O) mode between 230 K and 300 K, where increases rather than decreases, as predicted by Equation (3), suggests a possible explanation if the coexistence of the monoclinic and tetragonal phases is considered. Thus, based on the previous discussion and supported by the results in the literature (Noheda et al., 2002; Li et al., 2006), the occurrence of the following monoclinic (M
The stability of the monoclinic phase at low temperatures and the phase coexistence in the MPB of the PMN-PT system has also been frequently discussed in the literature. The phase coexistences in this system on zero-field cooling were considered in recent experimental works by using neutron diffraction, high-resolution X-ray diffraction and dielectric analysis (Singh & Pandey, 2006; Li et al., 2006). These studies have discussed the possibility of
tetragonal-monoclinic (T-MC) and tetragonal-monoclinic (T-MB) phase coexistence in unpoled PMN-PT ceramics in a wide temperature range. From these studies, the metastable phase diagram for this system in the MPB (see Fig. 7 in Li et al., 2006) was constructed based on the arguments that the (T-MB) phase coexistence is a non-equilibrium state and is the result of a local stress field and clampdown and blocking effect. A more recent study on the heterophase structures and the domain state-interface in the PMN-PT system, including the intermediate monoclinic phases (MB or MC), provides insight into understanding the stress-relief conditions at the phase coexistence near the MPB (Topolov, 2009). A correlation between the domain structures and the unit-cell parameters of adjacent MB and MC phases in certain temperature ranges could be suggested as the possible origin of the different sequences of phase transitions in solid solutions near the MPB.
3.2. The origin of the morphotropic phase boundary
To explain the large piezoelectric and electromechanical coupling coefficients observed in ferroelectric systems that exhibit an MPB, a polarization rotation model was proposed (Fu & Cohen, 2000; Guo et al., 2000). A giant piezoelectric response has been observed for Pb(Zn1/3Nb2/3)O3-PbTiO3 (PZN-PT) and PMN-PT single crystals in the rhombohedral phase, which have a polarization along the  direction. The crystals respond mechanically with a remarkable increase in strain if a small electric field is applied along the (001) direction. However, when the magnitude of the electric field is increased, a very flat strain-versus-field slope is observed (Fu & Cohen, 2000; Park & Shrout, 1997). Thus, the giant piezoelectric response could be explained by the reorientation of the polar domains, which depends on the mesoscopic structure or ordering, or by the polarization rotation mechanism at the atomic level (Fu & Cohen, 2000). An intuitive explanation for this mechanism can be delineated based on fact that PbTiO3 is a ferroelectric, which does not present a rhombohedral phase, with a large strain level of 6%. However, if there were a rhombohedral phase in PbTiO3, a colossal mechanical strain would be induced by applying an electric field. The model was proposed based on first-principles calculations on the classical BaTiO3 ferroelectric perovskite, by selecting different polarization directions and calculating their internal energies, provided explanations for the experimental observations (Park & Shrout, 1997; Park et al., 1999). Bellaiche et al. (Bellaiche et al., 2000) have succeeded in deriving the monoclinic phase of the PZT system at compositions around the MPB from first-principles calculations, showing that the predicted structural data were in good agreement with the measurements and consistent with the monoclinic phase as an intermediate phase between the tetragonal and rhombohedral phases.
The proposed polarization vector rotation for monoclinic phases in the PMN-PT system is schematically illustrated in Fig. 1-B. As the monoclinic phase represents the structural bridge between the tetragonal (space group P4mm) and rhombohedral (space group R3m) phases, the symmetry constrains the polarization vector to remain in the monoclinic plane, but is free to rotate within it (Noheda, 2002). The polarization vector of the MC phase can rotate along the ac plane between the (001) and (101) directions, while the MB phase can rotate along the bc plane between the (101) and (111) directions, configuring the polarization rotation model. The rotation of the polarization vector along these planes is responsible for the high values observed for the piezoelectric coefficients d
The revision of results and traditional notions acquired about ferroelectrics in the past few decades has led to new ideas and interpretations, demanding new experiments and models to explain the nature of the MPB (Kreisel et al., 2009; Khachaturyan, 2010). Some partial conclusions indicate that the MPB is considered more of a region than a boundary, characterized by two competing coexisting phases. However, some points still remain unclear to explain the giant electromechanical response of ferroelectric solid solutions near the MPB. The apparent violation of the Landau theory of the second-order phase transition, which does not permit a gradual rotation of the polarization vector under an applied electric field in the monoclinic phase, since the transition between different monoclinic phases is expected to occur, has resulted in alternative propositions to explain the phenomenology in the MPB (Khachaturyan, 2010). If the monoclinic phase is considered an adaptive phase, however, an adaptive state can be assumed in the MPB, and thus, gradual polarization rotation is now possible because of the easy rearrangement of nanodomains under the reduced polar anisotropy. The theory of an adaptive phase was developed to predict the ferroelectric transitions in solid solutions near the MPB and is based on stress-accommodating nanotwins domains (Jin et al., 2003; Bhattacharyya et al., 2008). The adaptive concepts have been extended to explain the origin of X-ray and neutron diffraction patterns of ferroelectric solid solutions systems near the MPB, but the existence of the monoclinic phase cannot be completely ruled out at low temperatures (Khachaturyan, 2010). These results demonstrate the necessity of additional experimental studies on traditional systems such as PZT and PMN-PT. The giant electromechanical response studied in PMN-PT single crystals was interpreted as a critical phenomenon such as in the electric-field–temperature–composition (E-T-x) phase diagram of PMN-PT a first-order paraelectric–ferroelectric phase transition terminates in a line of critical points where the piezoelectric coefficient is the maximum (Kutnjak et al., 2006). In addition, the large piezoelectric response observed at PMN-PT relaxors could be also related to the competition between ordered states at nanoscale in the presence of disorder and to the fact that any weak stress or electric field strongly affects such competition (Dkhil et al., 2009). All this work has provided valuable contributions to understanding the phenomenology behind the MPB.
Exploring theoretical predictions and experimental results for the similar MPB in the pure lead titanate PbTiO3, which appear under high hydrostatic pressure and cryogenics temperatures leading to tetragonal monoclinic rhombohedral phase transition, a more general idea of the morphotropic phase boundary could be introduced with perspectives of developing new high-performance electromechanical materials based on the chemical pressure idea (Ahart et al., 2008). In addition to these very attractive possibilities, observation of a low-symmetry monoclinic phase in the PbTiO3 opened very recent discussions on the arguments that justify the origin of morphotropic phase boundaries in ferroelectrics (Ahart et al., 2008) and arguments against the validity of the rotation polarization model to describe the stability of the phases and the sequence of phase transformation in the MPB in pure PbTiO3 (Frantti et al., 2008). This controversy is very interesting because the discussions illustrate how different ideas promote the advancement of science, showing the richness behind the research in phase transitions of systems that exhibit the MPB and that this subject is still open to new contributions.
Most modern piezoelectric materials used for technological applications are solid solutions that display a transition region in their composition-temperature phase diagrams, known as the morphotropic phase boundary, where the structure changes abruptly and the electromechanical properties exhibit maximal values. Some composition of PMN-PT ceramics, which are simpler to prepare than single crystals, is frequently used for technological applications due to their very high piezoelectric coefficient and electromechanical coupling coefficients. A major problem concerning the application of these electroceramics is the difficulty in producing a pyrochlore-free perovskite structure. Therefore, to prepare high-quality pyrochlore-free PMN-PT ceramics, several methods have been developed over the past three decades. In addition to the technological interest, the scientific comprehension of the origin of the morphotropic phase boundary in these ferroelectric solid solutions was a great challenge in past decades. The discovery of a stable monoclinic phase in the PZT system provides a new perspective to explain the high piezoelectric response of ferroelectric ceramics. The subsequent experimental and theoretical studies provided valuable contributions to understanding the phenomenology behind the MPB and promoted a significant advancement in the area. However, recent new ideas about and interpretations of the structural phase transition in high-performance ferroelectric systems and the nature of the MPB demonstrated that this subject is still open for discussion.
The author is grateful to Brazilian agencies FAPESP, CNPq and CAPES for the financial support for the correlated research. My special thanks to Pró-Reitoria de Pós-Graduação da UNESP (PROPG) and Fundação para o Desenvolvimento da UNESP (FUNDUNESP) for their financial support for this work.
Ahart M. et al. 2008Origin of morphotropic phase boundaries in ferroelectrics. 451 545 549 0028-0836
Araújo E. B. et al. 2007Synthesis of slightly <111>-oriented 0.65Pb(Mg1/3Nb2/3)O3-0.35PbTiO3 ceramic prepared from fine powders. 104 40 43 0254-0584
Araújo E. B. et al. 2008Structural phase transition studies on PMN-0.35PT using Infrared Spectroscopy. 369 35 42 1563-5112
Arigur P. Benguigui L. 1975Direct determination of coexistence region in solid-solutions Pb(ZrxTi1-x)O3. 8 1856 1862 1361-6463
Babooram K. et al. 2004Phase formation and dielectric properties of 0.90Pb(Mg1/3Nb2/3)O3-0.10PbTiO3 ceramics prepared by a new sol-gel method. 30 1411 1417 0272-8842
Baek J. G. et al. 1997Synthesis of pyrochlore-free 0.9Pb(Mg1/3Nb2/3)O3-0.1PbTiO3 ceramics via soft mechanochemical route. 80 973 981 1551-2916
Bellaiche L. et al. 2000Finite-Temperature properties of Pb(Zr1-xTix)O3 alloys from first principles. 84 5427 5430 1079-7114
Bhattacharyya S. et al. 2008Direct high-resolution transmission electron microscopy observation of tetragonal nanotwins within the monoclinic MC phase of Pb(Mg1/3Nb2/3)O3-0.35PbTiO3 crystals. 92 1429041 1429043 1077-3118
Bokov A. A. Ye Z. G. 2004Domain structure in the monoclinic Pm phase of Pb(Mg1/3Nb2/3)O3-PbTiO3 single crystals. Journal of Applied Physics 95 6347 6359 1089-7550
Bokov A. A. Ye Z. G. 2006Recent progress in relaxor ferroelectrics with perovskite structure 41 31 52 1573-4803
Chen K. P. et al. 2002Electric-field-induced phase transition in <001>-oriented Pb(Mg1/3Nb2/3)O 3PbTiO3 single crystals. 14, L571-L576. 0136-1648X
Chen S. Y. Chen I. W. 1994Temperature-time texture transition of Pb(Zr1−xTix)O3 thin films: II, Heat treatment and compositional effects. 77 2337 2344 1551-2916
Choi S. W. et al. 1989Morphotropic phase boundary in Pb(Mg1/3Nb2/3)O3-PbTiO3 system. 8 253 255 0016-7577X
Cruz L. P. et al. 2002An easy way to Pb(Mg1/3Nb2/3)O3 synthesis. 37 1163 1173 0025-5408
Dkhil B. et al. 2009Intermediate temperature scale T* in lead-based relaxor systems. 80 064103 064109 0155-0235x
Du X. J. et al. 1998Crystal orientation dependence of piezoelectric properties of lead zirconate titanate near the morphotropic phase boundary. 72 2421 2423 1077-3118
Frantti J. et al. 2008Evidence against the polarization rotation model of piezoelectric perovskites at the morphotropic phase boundary. 20 472203 472203 0136-1648X
Fu H. X. Cohen R. E. 2000Polarization rotation mechanism for ultrahigh electromechanical response in single-crystal piezoelectrics. 403 281 283 0028-0836
Guerra J. D. S. et al. 2009Investigation on dielectric response of PMN ceramics around paraelectric-ferroelectric diffuse phase transition. 25 1316 1320 1743-2847
Gu H. et al. 2003Single-calcination synthesis of pyrochlore-free 0.9Pb(Mg1/3Nb2/3)O3-0.1PbTiO3 and Pb(Mg1/3Nb2/3)O3 ceramics using a coating method. 86 217 221 1551-2916
Guo R. et al. 2000Origin of the high piezoelectric response in PbZr1-xTixO3. Physical Review Letters 84 5423 5426 1079-7114
Hatch D. M. et al. 2002Antiferrodistortive phase transition in Pb(Ti0.48Zr0.52)O3: Space group of the lowest temperature monoclinic phase. Physical Review B 65 212101 212103 0155-0235x
Hlinka J. et al. 2006Infrared dielectric response of relaxor ferroelectrics. 79 41 78 1029-0338
Hlinka J. et al. 2006Anisotropic dielectric function in polar nanoregions of relaxor ferroelectrics. 96 027601 027604 1079-7114
Johnson D. W. 1985Sol-gel processing of ceramics and glass. 64 1597 1602 1551-2916
Jin Y. M. et al. 2003Adaptive ferroelectric states in systems with low domain wall energy: Tetragonal microdomains. 94 3629 3640 1089-7550
Kamba S. et al. 2007Quantum paraelectric behavior of pyrochlore Pb1.83Mg0.29Nb1.71O6.39. 76 054125 054131 0155-0235x
Kakegawa K. Mohri J. 1977A compositional fluctuation and properties of Pb(Zr,Ti)O3. 24 769 772 0038-1098
Kelly J. et al. 1997Effect of composition on the electromechanical properties of (1-x)Pb(Mg1/3Nb2/3)O3-xPbTiO3 ceramics. 80 957 964 1551-2916
Khachaturyan A. G. 2010Ferroelectric solid solutions with morphotropic boundary: Rotational instability of polarization, metastable coexistence of phases and nanodomain adaptive states. 90 37 60 1478-6443
Kong L. B. et al. 2001Preparation of PMN powders and ceramics via a high-energy ball milling process. 20 1241 1243 1573-4811
Kreisel J. et al. 2009Phase transitions and ferroelectrics: revival and the future in the field. Phase Transitions 82 633 661 1029-0338
Kutnjak Z. et al. 2006The giant electromechanical response in ferroelectric relaxors as a critical phenomenon. 441 956 959 0028-0836
Kwon S. et al. 2005High strain, <001> textured 0.675Pb(Mg1/3Nb2/3)O3-0.325PbTiO3 ceramics: Templated grain growth and piezoelectric properties. 88 312 317 1551-2916
Last J. T. 1957Infrared-absorption studies on barium titanate and related materials. 105 1740 1750 1536-6065
Li J. B. et al. 2006Structural transition in unpoled (1-x)PMN-xPT ceramics near the morphotropic boundary. 425 373 378 0925-8388
Mergen A. Lee W. E. 1997Fabrication, characterisation and formation mechanism of Pb1.83Mg0.29Nb1.71O6.39 pyrochlore. 17 1033 1047 0955-2219
Mishra S. K. et al. 1996Effect of phase coexistence at morphotropic phase boundary on the properties of Pb(ZrxTi1−x)O3 ceramics. 69 1707 1709 1077-3118
Noblanc O. et al. 1996Structural and dielectric studies of Pb(Mg1/3Nb2/3)O3-PbTiO3 ferroelectric solid solutions around the morphotropic boundary. 79 4291 4297 1089-7550
Noheda B. et al. 1999A monoclinic ferroelectric phase in the Pb(Zr1-xTix)O3 solid solution 74 2059 2062 1077-3118
Noheda B. et al. 2001Tetragonal-to-monoclinic phase transition in a ferroelectric perovskite: The structure of PbZr0.52Ti0.48O3. B 61 8687 8695 0155-0235x
Noheda B. et al. 2001Stability of the monoclinic phase in the ferroelectric perovskite PbZr1-xTixO3. B 63 014103 014112 0155-0235x
Noheda B. et al. 2002Phase diagram of the ferroelectric relaxor (1-x)PbMg1/3Nb2/3O3-xPbTiO3. 66 054104 054114 0155-0235x
Noheda B. 2002Structure and high-piezoelectricity in lead oxide solid solutions. 6 27 34 1359-0286
Noheda B. Cox D. E. 2006Bridging phases at the morphotropic boundaries of lead oxide solid solutions. 79 5 20 1029-0338
Panda P. K. Sahoo B. 2005Preparation of pyrochlore-free PMN powder by semi-wet chemical route. 93 231 236 0254-0584
Pandey D. Ragini 2003On the discovery of new low temperature monoclinic phases with Cm and Cc space groups in Pb(Zr0.52Ti0.48)O3: an overview. 218 1 7 0044-2968
Pandey D. et al. 2008Stability of ferroic phases in the highly piezoelectric Pb(Zr,Ti)O3 ceramics. 64 192 203 0108-7673
Park S. E. Shrout T. R. 1997Characteristics of relaxor-based piezoelectric single crystals for ultrasonic transducers. 44 1140 1147 0885-3010
Pechini M. 1967Method of preparing lead and Al-alkaline-earth titanates and niobates and coating method using the same to form a capacitor. U.S. Pat. N° 3 330 697.
Perry C. H. et al. 1964Infrared studies of perovskite titanates. 135, A 408A412. 1536-6065
Randall C. A. et al. 1998Intrinsic and extrinsic size effects in fine-grained morphotropic-phase-boundary lead zirconate titanate ceramics. 81 677 688 1551-2916
Ranjan R. et al. 2002Antiferrodistortive phase transition in Pb(Ti0.48Zr0.52)O3: A powder neutron diffraction study. 65 060102 060106 0155-0235x
Ranjan R. et al. 2005Comparison of the Cc and R3c space groups for the superlattice phase of Pb(Zr0.52Ti0.48)O3. B 71, 092101-092104 (2005). 0155-0235 1550 235x
Sabolsky E. M. et al. 2001Piezoelectric properties of <001> textured Pb(Mg1/3Nb2/3)O3-PbTiO3 ceramics. 78 2551 2553 1077-3118
Sekar M. M. A. Halliyal A. 1998Low-temperature synthesis, characterization, and properties of lead-based ferroelectric niobates. 81 380 388 1551-2916
Shrout T. R. Swartz S. L. 1983Dielectric-properties of pyrochlore lead magnesium niobate. 18 663 667 0025-5408
Singh A. K. Pandey D. 2001Structure and the location of the morphotropic phase boundary region in ( 1x)[Pb(Mg1/3Nb2/3)O3]-xPbTiO3. 13, L931-L936. 0136-1648X
Singh A. K. et al. 2002Powder neutron diffraction study of phase transitions in and a phase diagram of (1-x)[Pb(Mg1/3Nb2/3)O3]-xPbTiO3. B 66 0541011 0241019 0155-0235x
Singh A. K. Pandey D. 2003Evidence for MB and MC phases in the morphotropic phase boundary region of (1-x)[Pb(Mg1/3Nb2/3)O3]-xPbTiO3: A Rietveld study. 67 064102 064114 0155-0235x
Singh A. K. Pandey D. 2006Powder neutron diffraction study of phase transitions in and a phase diagram of (1-x)[Pb(Mg1/3Nb2/3)O3]-xPbTiO3. 74 024101 024119 0155-0235x
Singh A. K. et al. 2007High-resolution synchrotron x-ray diffraction study of Zr-rich compositions of Pb(ZrxTi1-x)O3 (0.525 ≤ x ≤ 0.60): Evidence for the absence of the rhombohedral phase. 91 192904 192907 1077-3118
Singh A. K. et al. 2008Origin of high piezoelectric response of Pb(ZrxTi1-x)O3 at the morphotropic phase boundary: Role of elastic instability. 92 022910 022913 1077-3118
Souza A. G. et al. 2000Monoclinic phase of PbZr0.52Ti0.48O3 ceramics: Raman and phenomenological thermodynamic studies. B 61 14283 14286 0155-0235x
Souza A. G. et al. 2002Raman scattering study of the PbZr1-xTixO3 system: Rhombohedral-monoclinic-tetragonal phase transitions. B 66 132107 132111 0155-0235x
Subramanian M. A. et al. 1983Oxide pyrochlores- A review. 15 55 143 0079-6786
Sun S. et al. 2004Fabrication and electrical properties of grain-oriented 0.7Pb(Mg1/3Nb2/3)O3-0.3PbTiO3 ceramics. 84 574 576 1077-3118
Swartz S. L. Shrout T. R. 1982Fabrication of perovskite lead magnesium niobate. 17 1245 1250 0025-5408
Swartz S. L. et al. 1984Dielectric properties of lead-magnesium niobate ceramics. 67 311 315 1551-2916
Spitzer W. G. et al. 1962Far infrared dielectric dispersion in BaTiO3, SrTiO3 and TiO2. 126 1710 1962 1536-6065
Topolov V. Yu 2009Monoclinic phases and stress-relief conditions in(1-x)Pb(Mg1/3Nb2/3)TiO3-xPbTiO3 solid solutions. 480 568 574 0925-8388
Isupov V. A. 1975Comments on the paper “x-ray study of the pzt solid solutions near the morphotropic phase transition”. 17 1331 1333 0038-1098
Viehland D. et al. 2001Piezoelectric instability in <011>-oriented Pb(B1/3IB2/3II)O3-PbTiO3 crystals. 79 1006 1009 1077-3118
Viehland D. et al. 2004Domain structure changes in (1-x)Pb(Mg1/3Nb2/3)O3-xPbTiO3 with composition, dc bias, and ac field. 96 3379 3381 1089-7550
Vanderbilt D. Cohen M. H. 2001Monoclinic and triclinic phases in higher-order Devonshire theory. 63 094108 094117 0155-0235x
Wang H. C. Schulze W. A. 1990The role of excess magnesium oxide or lead oxide in determining the microstructure and properties of lead magnesium niobate. 73 825 832 1551-2916
Woodward D. I. et al. 2005Review of crystal and domain structures in the PbZrxTi1-xO3 solid solution. 72 104110 04118 0155-0235x
Ye Z. G. Dong M. 2000Morphotropic domain structures and phase transitions in relaxor-based piezo-/ferroelectric (1-x)Pb(Mg1/3Nb2/3)O3-xPbTiO3 single crystals. 87 2312 2320 1089-7550
Ye Z. G. et al. 2001Monoclinic phase in the relaxor-based piezoelectric/ferroelectric Pb(Mg1/3Nb2/3)O3-PbTiO3 system. 64 184114 184119 0155-0235x
Yokota H. et al. 2009Crystal structure of the rhombohedral phase of PbZr1−xTixO3 ceramics at room temperature. 80 104109 104121 0155-0235x
Yoon K. H. et al. 1995Characteristics of lead magnesium niobate thin-film prepared by sol-gel processing using a complexing agent. 78 2267 2270 1551-2916
Zhao X. Y. et al. 2003Effect of a bias field on the dielectric properties of 0.69Pb(Mg1/3Nb2/3)O3-0.31PbTiO3 single crystals with different orientations. 15 6899 6908 0136-1648X